| ||Format||Pages||Price|| |
|5||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$44.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$52.80||  ADD TO CART|
Significance and Use
5.1 Controlled stimulation i.e. the application of mechanical or thermal load, can generate AE from flawed areas of the structure. Sources may include flaw growth, oxide fracture, crack face stiction and release on load application, and crack face rubbing.
5.2 The load range above normal service (peak) load is used to propagate fatigue cracks in the plastically strained region ahead of the crack tip. Crack propagation may not be a reliable source of AE, depending on the alloy and microstructure, the amount (rate) of crack extension, and possibility of brittle fracture in a segment of crack extension.
5.3 Load increases resulting in significant ductile tearing may produce less emission than expected for the amount of crack growth. Processes that result in more brittle cleavage fractures are more detectable and produce more emission for smaller amounts of flaw growth. These include corrosion fatigue and stress corrosion cracking modes of flaw growth, and would also be more likely in cast or welded structures than in fabricated (forged, rolled or extruded) structures. Distributed defect structures such as hydrogen embrittlement, or creep cavitation in high temperature steels may also produce significant emission without evidence of an existing crack-like flaw.
5.4 Application and relaxation of load can produce secondary mechanically-induced emission that is not related to flaw extension. This includes crack face stiction release on loading—usually evidenced by emission at the same rising load value regardless of peak load; or crack face rubbing on load release as the fracture surfaces come back together.
1.1 This practice provides guidelines for acoustic emission (AE) monitoring of structures, such as pressure vessels, piping systems, or other structures that can be stressed by mechanical or thermal means.
1.2 The basic functions of an AE monitoring system are to detect, locate, and classify emission sources. Other methods of nondestructive testing (NDT) may be used to further evaluate the significance of reported acoustic emission sources.
1.3 Units—The values stated in either SI units or inch-pound units are to be regarded as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standards.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E543 Specification for Agencies Performing Nondestructive Testing
E650 Guide for Mounting Piezoelectric Acoustic Emission Sensors
E750 Practice for Characterizing Acoustic Emission Instrumentation
E1316 Terminology for Nondestructive Examinations
E2374 Guide for Acoustic Emission System Performance Verification
Other DocumentsANSI/ASNT CP-189 Standard for Qualification and Certification of Nondestructive Testing Personnel
AIA StandardNAS-410 Certification and Qualification of Nondestructive Testing Personnel Available from Aerospace Industries Association of America, Inc. (AIA), 1000 Wilson Blvd., Suite 1700, Arlington, VA 22209-3928, http://www.aia-aerospace.org.
ICS Number Code 91.120.20 (Acoustics in buildings. Sound insulation)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E569 / E569M-13, Standard Practice for Acoustic Emission Monitoring of Structures During Controlled Stimulation, ASTM International, West Conshohocken, PA, 2013, www.astm.orgBack to Top